### Version: Accepted Version

**Proceedings Paper:**

### Houghton, M orcid.org/0000-0003-3244-5699, Head, D orcid.org/0000-0003-0216-6787

### and Walkley, M orcid.org/0000-0003-2541-4173 (2019) A Numerical Model for Random

### Fibre Networks. In: Nikolov, G, Kolkovska, N and Georgiev, K, (eds.) Lecture Notes in

### Computer Science. 9th International Conference on Numerical Methods and Applications

### (NMA 2018), 20-24 Aug 2018, Borovets, Bulgaria. Springer , pp. 408-415. ISBN

### 978-3-030-10691-1

### https://doi.org/10.1007/978-3-030-10692-8_46

### © 2019, Springer Nature Switzerland AG. This is a post-peer-review, pre-copyedit version

### of an article published in Lecture Notes in Computer Science. The final authenticated

### version is available online at: https://doi.org/10.1007/978-3-030-10692-8_46. Uploaded in

### accordance with the publisher's self-archiving policy.

eprints@whiterose.ac.uk
https://eprints.whiterose.ac.uk/
**Reuse **

Items deposited in White Rose Research Online are protected by copyright, with all rights reserved unless indicated otherwise. They may be downloaded and/or printed for private study, or other acts as permitted by national copyright laws. The publisher or other rights holders may allow further reproduction and re-use of the full text version. This is indicated by the licence information on the White Rose Research Online record for the item.

**Takedown **

If you consider content in White Rose Research Online to be in breach of UK law, please notify us by

## A Numerical Model For Random Fibre Networks

Mark Houghton⋆[0000−0003−3244−5699]_{, David Head}[0000−0003−0216−6787]_{, and}

Mark Walkley[0000−0003−2541−4173]

University Of Leeds, Leeds, UK

Abstract. Modelling a random fibre network representative of a real world material leads to a large sparse linear matrix system with a high condition number. Current off-lattice networks are not a realistic model for the mechanical properties of the large volume of random fibres seen in actual materials. In this paper, we present the numerical methods em-ployed within our two-dimensional and three-dimensional models that improve the computational time limitations seen in existing off-lattice models. Specifically, we give a performance comparison of two-dimensional random fibre networks solved iteratively with different choices of precon-ditioner, followed by some initial results of our three-dimensional model.

Keywords: Fibre network·_{Iterative}·_{Preconditioning.}

### 1

### Introduction

Many real world materials can be represented at the microscopic level by a random network of fibres, including paper and felt, non-woven fabrics, tissue scaffolds, and the cytoskeletons of eukaryotic cells. A good understanding of the mechanical behaviour of these networks is key to understanding physical properties at the macroscopic level and for the development of new materials.

### 2

### Modelling a Random Fibre Network

In many applications, especially biological, it is appropriate to model individual fibres as semiflexible polymers [5]. With this assumption in place, the extensible

Wormlike Chain model has been shown to adequately describe the elastic be-haviour of individual semiflexible fibres [6]. Discretising this we can define fibre stretching, compression and bending, but we choose to neglect thermal contribu-tions for simplicity. To expand this theory from single fibres to whole networks we adopt the Mikado model [3, 4, 7], which allows us to express the energy of the system as the total sum of stretching energy added to the total sum of bending energy of the network,

E=µ 2

X

ij

δℓ2_{ij}
ℓij

+1 2

X

hijki

κijkθijk2 ¯

ℓijk

, (1)

2 M. Houghton et al.

where the left sum considers all segments,ij, of every fibre of the network, and the right sum considers all of the consecutive segments,ij,jk, along each fibre, for stretching constant µ, bending modulus κijk, segment length ℓij, average length of two consecutive segments ¯ℓijk, and angular deflectionθijk. To better understand (1), it is useful to first consider individual fibres.

2.1 Fundamentals

Defining fibres as slender elastic bodies with uniform circular cross-sections, we can consider a two-dimensional plane or three-dimensional cuboid wherein a predetermined number of fibres are generated with random position and orien-tation. After cross-linking these fibres (see 2.5), a mechanical structure remains in which nodes are identified as freely rotating points, and categorised as one of three types. Boundary nodes occur as points fixed at the aperiodic boundaries of the domain, dangling nodes are attributed to the end points of fibres not on the boundary, and internal nodes are the points associated with cross-links. For adjacent nodesϕ,ψ the tangent vector along the segment is

ˆ_{t}_{ϕψ}_{=} sψ−sϕ

ℓϕψ

,

wheresϕis the position vector at ϕand ℓϕψ=|sψ−sϕ|is the segment length. We denoteuϕ as the displacement of an individual node after a load or pertur-bation has been applied to the network, and refer to individual components as

uϕx, uϕy, uϕz.

2.2 Local Stretching Behaviour

Consider a segmentϕψ comprising of an adjacent node pair ϕ, ψ respectively, treated as a simple Hookean spring. The stretching energy for this segment is

Eϕψstretch=

kϕψ

2 [(uψ−uϕ)·ˆtϕψ]

2

with a stretching constantkϕψ=_{ℓ}_{ϕψ}µ = AE
f

ℓϕψ , forA=πr

2_{, radius}_{r}_{and Young’s}

modulus Ef_{. The second partial derivatives of this energy contribute to the}
global Hessian matrix at rows and columns corresponding to the displacements
of ϕ and ψ, and the first partial derivatives contribute to the right hand side
vector.

2.3 Local Bending Behaviour

For the adjacent node tripletα, ω, β, segmentαωβhas bending energy

Eαωβbend=

καωβθ2αωβ 2¯ℓαωβ

=καωβ[(sω−sα)×(uβ−uω) + (uω−uα)×(sβ−sω)]

2

ℓ2

αωℓ2ωβ(ℓαω+ℓωβ)

,

for a bending constantκαωβ = AE f

r2

4 , withA=πr2and Young’s modulus Ef.

2.4 Global Assembly

Combining the displacementsuϕ of every nodeϕ, in the vectorU,

U= [U1, U2, U3, U4, ...] = [u1x, u2x, ..., u1y, u2y, ..., u1z, u2z, ...],

then a Taylor series expansion of the energy of the system aboutU= 0 is

E(U) =E0+

N
X
i=1
Ui
∂E
∂Ui
_{U}_{=}_{0}

+1 2 N X i=1 N X j=1

UiUj

∂2_{E}

∂Ui∂Uj
_{U}_{=}_{0}

+ ...

The resulting system represents the network in mechanical equilibrium with the applied load or perturbation;

X

j

Uj

∂2_{E}

∂Ui∂Uj

=Bi, whereBi=−

∂E
∂Ui
_{U}
=0

fori, j= 1, ..., N. Denoting the Hessian matrix asH, this gives the global linear matrix system HU = B which can be assembled from the local contributions defined in sections 2.2 and 2.3.

2.5 Cross-linking Fibres

In a two dimensional plane, a pair of randomly orientated fibres are trivially
cross-linked at their unique point of intersection, if this exists. In three
dimen-sions direct intersections of randomly orientated fibres occur with probability
zero for radius,r→0+_{. In this case, the minimum separation is considered, and}

if this is below a given threshold, a short cross-linking fibre is inserted between the two closest points of the original pair of fibres. The cross-linking fibre can either be treated as a stiff and non-rotating inextensible rod, in which case each end point displaces identically, or as an elastic spring, in which case each end point can displace individually. An alternative approach is to constrain fibre orientation to lie along lattice vectors, such that fibres directly intersect. This lattice-based approach can achieve mechanical rigidity at lower fibre counts due to the higher coordination (connectivity) number, zc, and has been used suc-cessfully to predict mechanical properties comparable to randomly orientated fibre networks seen in real-world materials [2]. We have made some preliminary lattice-based experiments (discussed in Section 4.3) before moving to randomly orientated networks.

### 3

### Numerical Model

3.1 Linear System Structure (in 2D)

By grouping the unknown displacements inUby coordinate direction, the block structure ofH can be written as

H =

HxxHxy

HT xy Hyy

, whereHϕψ=

∂2E ∂uϕi∂uψj

4 M. Houghton et al.

fori, j= 1, ..., N.

The sparsity of H is determined from the local connectivity of each fibre with the other fibres in the network. An initial estimate of the sparsity pattern can be obtained from the adjacency matrix of the internal nodes of a network, and is repeated for each sub-blockHϕψ of the global matrixH. To exploit the sparsity of H, we store the non-zero values in compressed sparse row (CSR) format. The matrixH is symmetric, as are each of the diagonal sub-blocks, but each off-diagonal sub-block is not necessarily symmetric.

3.2 Iterative Solution Strategy

Our system is symmetric but may not be positive definite, hence we choose the MINRES iterative method from the family of Krylov subspace methods. These methods perform best when the system is preconditioned to cluster the matrix eigenvalues. Exploiting the block structure seen in (2), we take the diagonal blocks

PDb=

Hxx O

O Hyy

, (3)

as the first choice of preconditioner. A similar preconditioner can be defined when extending to three dimensions. Additionally we can also consider a simple asym-metric preconditioner and a symasym-metric preconditioner with a Schur complement block

PAb=

HxxHxy

O Hyy

, PS =

HxxO

O S

, (4)

whereS =Hyy−HxyT Hyy−1Hxy. GMRES was used with PAb, since this precon-ditioner does not preserve the symmetry ofH.

### 4

### Results

4.1 Performance Comparison in 2D

To evaluate the performance of the different choices of preconditioner, we
mea-sured the number of iterations required to converge to a relative tolerance of
10−3_{, using the MINRES and GMRES solvers in MATLAB. The rate of }

con-vergence was measured for increasing system size by increasing the number of fibres,Nf, with fixed length ℓ= 0.25 and radius r= 0.01. For each interval of

Nf, the results were averaged over 10 reproducibly-seeded randomly generated networks. Examples of individual network generations with varying Nf can be seen in Figure 1.

Fig. 1. Examples of generated 2D random fibre networks increasing in area with a fixed fibre density. The number of fibres,Nf, is 100(left), 400 and 1600 (right), and

fibre length,ℓ, and radius,r, are fixed at 0.25 and 0.01 respectively, but r is not to scale. Dangling ends have not been removed.

diagonally scaled preconditioner D performs the worst, with large fluctuations in the iteration count and a large standard error.

Table 1.Number of iterations required to converge for different preconditioners and an increasing number of fibres,Nf, of length 0.25 and radius 0.01. Standard error was

calculated from a sample of 10 networks.

Nf 100 200 400 800

D 300.2±_{54}_{.}_{0} _{480}_{.}_{8}±_{67}_{.}_{3} _{570}_{.}_{6}±_{77}_{.}_{3} _{410}_{.}_{9}±_{103}_{.}_{0}
PDb 8.0±0.8 8.5±0.5 7.7±0.7 7.2±0.6

PS 12.3±1.1 14.6±1.2 13.8±1.3 14.1±0.9

PAb 5.3±0.2 5.4±0.2 5.4±0.2 5.3±0.2

As a further indication of performance we also collected estimates for the condition numbers of the preconditioned system and forH. To do this we con-sider a similar range of Nf as previously and provided the default seed to the

condest_{function in MATLAB for 10 network generations at each interval. From}

the results in Table 2 we find additional evidence for the poor performance of

D, with condition number estimates consistently higher than H without any preconditioning.PS reduces the condition number ofH by roughly an order of magnitude, andPDb andPAb demonstrate the best performance, showing simi-lar estimates to each other with the symmetric having slightly lower values on average for largerNf.

ener-6 M. Houghton et al.

Table 2.Estimated condition numbers, κ, of different preconditioners applied toH, for varied number of fibres,Nf.

Nf 100 200 400 800 1600

κ(H) 3.74e6 7.58e6 1.81e7 4.34e7 9.72e7
κ(D−1_{H}_{)} _{8.51e6} _{2.41e7} _{7.09e7} _{1.98e8} _{4.54e8}

κ(P−1

DbH) 7.32e4 1.47e5 4.85e5 1.60e6 5.12e6

κ(P−1

S H) 1.39e5 4.97e5 1.18e6 4.22e6

-κ(P−1

AbH) 6.98e4 1.96e5 5.99e5 2.11e6

-10-2 10-1

0.4 0.5 0.6 0.7 0.8 0.9 1 1.1

10-2 10-1

0.1 0.15 0.2 0.25

Fig. 2.r/ℓ, forℓ= 0.25 and Nf = 100 in a 0.5×0.5 plane againstG/Gaff (left)and

againstEb_{/E}_{(right)}_{. Nodes within a distance of 10}−3 _{were merged into a single node}

prior to solution. The lineG/Gaff

= 1 (left) corresponding to affine response is also shown.

100 200 400 800 1600

10-6 10-5

100 200 400 800 1600

0 1 2 3 4

5 10

-3

gies for small r, to a stretching dominated regime for large r. Figure 2 (left)

demonstrates a smooth transition between affine (i.e. uniform deformation field) dominated behaviour at large r to non-affine behaviour for small r. This co-incides well with the known result that stretching-dominated networks become close to affine [4].

4.2 Validation

To validate our model results, we verified that the calculated energy,E, and shear
modulus, G, were bounded by the affine predictions Eaff _{and} _{G}aff _{respectively.}

To do this, we increasedNf for ℓ = 0.25 and r = 0.01, and plotted E and G alongside their corresponding affine predictions. Figure 3 demonstrates thatE

(left) and G(right) lie below the limits provided by the affine predictions. We can also see thatEincreases linearly withNf, as we would expect.

4.3 Preliminary Results in 3D

In a step towards solving randomly orientated three dimensional networks built from the Mikado approach, we were able to obtain preliminary results by solving networks with predetermined direct intersections between fibres. These have irregularity introduced by overlaying different lattice based components together to form a rigid structure. More specifically we take 25 vertical fibres extending the height of a 1×1×1 cube and insert lattice forming plates through the vertical fibres with varied orientations.

Fig. 4. Visualisations of one of the lattice based 3D networks, for the undisplaced

(left), displaced(centre)and affinely displaced(right)generations of the network where γ= 0.05.

8 M. Houghton et al.

the structure prior to any shear, Figure 4(centre)shows the structure displaced after shearing, where the displacements are calculated using a direct solver. Figure 4(right)shows the structure with every node displaced affinely. The total energy in this case isEtotal

aff = 5.0e−7. Comparing(centre) and(right), we can

see regions of the network in(centre) where bending is more favourable than
affine displacement. The total energy here is Etotal _{= 1}_{.}_{4}_{e}−7_{, where bending}

energyEbend = 1.3e−7is the main contribution.

### 5

### Continued Work

Although lattice-based modelling can provide valuable insight into the mechan-ical properties of random fibre networks, truly representing real-world materials is still an issue. This will require a model with genuinely random orientation, using one of the two approaches for minimum distance calculation discussed in Section 2.5.

The size of the linear system becomes significant in 3D and parallel comput-ing will be essential to model realistic volumes of material. We intend to use PETSc [1] to develop scalable tools for solving our systems, employing the block preconditioned iterative methods demonstrated in Section 4.1.

### References

1. Balay, S., Abhyankar, S., Adams, M., Brown, J., Brune, P., Buschelman, K., Dalcin, L., Eijkhout, V., Gropp, W., Kaushik, D., Knepley, M., May, D., McInnes, L., Mills, R., Munson, T., Rupp, K., Sanan, P., Smith, B., Zampini, S., Zhang, H., Zhang, H.: PETSc Web page (2018), http://www.mcs.anl.gov/petsc

2. Broedersz, C., Mao, X., Lubensky, T., MacKintosh, F.: Criticality and isostaticity in fibre networks. Nature Physics7(12), 983–988 (2011)

3. Head, D., MacKintosh, F., Levine, A.: Nonuniversality of elastic exponents in ran-dom bond-bending networks. Phys. Rev. E68(2), 25101 (2003)

4. Head, D., Levine, A., MacKintosh, F.: Deformation of Cross-Linked Semiflexible Polymer Networks. Physical Review Letters91(10), 108102 (2003)

5. MacKintosh, F.: Elasticity and dynamics of cytoskeletal filaments and their net-works. In: Soft condensed matter physics in molecular and cell biology, pp. 139–145. Taylor & Francis (2006)

6. Storm, C., Pastore, J., MacKintosh, F., Lubensky, T.C., Janmey, P.: Nonlinear elasticity in biological gels. Nature435(7039), 191 (2005)